Measurement of stresses in the vibrating elements of a printing device
V. Bivainis^{1} , E. Kibirkštis^{2} , L. Gegeckienė^{3} , V. Miliūnas^{4} , N. Buškuvienė^{5} , L. Ragulskis^{6}
^{1}Aleksandras Stulginskis University, Studentų str. 11, LT53361 Akademija, Kaunas District, Lithuania
^{2, 3, 4, 5}Kaunas University of Technology, Department of Graphic Communication Engineering, Studentų str. 56350, LT51424 Kaunas, Lithuania
^{6}Vytautas Magnus University, Vileikos 8, 44404 Kaunas, Lithuania
Journal of Vibroengineering, Vol. 15, Issue 4, 2013, p. 20222028.
Received 24 October 2013; accepted 25 October 2013; published 31 December 2013
JVE Conferences
In this paper measurement of stresses in vibrating elements of the printing device using photoelastic techniques is investigated. Numerical procedure is applied to obtain data which is needed for the interpretation of experimental results of time averaged photoelasticity when sinusoidal vibrations according to the eigenmode of the structure in the problem of plane stress take place. The results obtained from this numerical procedure correspond with the results obtained analytically earlier. The numerical procedure is also applied to obtain data which is needed for interpretation of experimental results when the structure is slowly loaded from the status of equilibrium by linearly increasing the load till its final value. Experimental measurements of stresses in polymeric films have been performed. Qualitative investigations of stresses of samples of LDPE films were performed by taking into account the level of stresses in unloaded samples as well as in samples experiencing tensile loading. Samples of LDPE films having various characteristics were analyzed. In order to obtain photoelastic images representing stress distributions in the investigated polymeric films the experimental setup was developed. In the loaded samples of the investigated films of LDPE type higher order photoelastic fringes are observed. They enable to interpret stress distributions in the films. This is especially important in the process of operation of the printing device. The obtained results are used in the process of measurements of stresses in the elements of a printing device.
Keywords: printing device, measurement of stresses, time averaging, photoelasticity, plane stress, eigenmodes, experimental setup, polymeric film, General Purpose Strain Viewer, digital camera, digital image.
1. Introduction
The investigations about time averaging in photoelasticity presented in this paper are based on the material presented in [1]. In this previous paper the data which is necessary to interpret experimental results of time averaged photoelasticity were obtained on the basis of analytical investigations based on manipulation of integrals and using the zeroth order Bessel function of the first kind. In this paper numerical procedure is applied to obtain data which is needed for the interpretation of experimental results of time averaged photoelasticity when sinusoidal vibrations according to the eigenmode of the structure in the problem of plane stress take place. The results obtained from this numerical procedure correspond with the results obtained analytically in the previous paper. The numerical procedure is also applied to obtain data which is needed for interpretation of experimental results when the structure is slowly loaded from the status of equilibrium by linearly increasing the load till its final value.
Some experimental findings of distribution of stresses in flat clear polymeric plates using photoelastic method of investigations are presented in the papers [210]. The authors mostly analyze the effect at melting, molding or cooling temperatures, pressure, time and other parameters to the level of stresses.
Experimental measurements of stresses in polymeric films have been performed. Qualitative investigations of stresses of samples of LDPE films were performed by taking into account the level of stresses in unloaded samples as well as in samples experiencing tensile loading. Samples of LDPE films having various characteristics were analyzed. In order to obtain photoelastic images representing stress distributions in the investigated polymeric films the experimental setup was developed. The basic part of the experimental setup is „General Purpose Strain Viewer“. Photoelastic images representing stress distributions were registered by using a digital camera.
In the loaded samples of the investigated films of LDPE type higher order photoelastic fringes are observed. They enable to interpret stress distributions in the films. This is especially important in the process of operation of the printing device. An experienced operator of the printing device from the typical photoelastic fringe patterns can judge about the distribution of stresses in the polymeric film. When the stresses become excessive and stress concentration takes place there is danger that the polymeric film may experience defects (residual strains and tears). Thus when the operator of the printing device notices from the photoelastic images that such a critical situation is approaching, he is to immediately stop the process of printing and make necessary adjustments.
The obtained results are used in the process of interpretation of stress measurements in photoelastic experiments and for measurement of stresses in the elements of a printing device.
2. Measurement of stresses in time averaged photoelasticity
2.1. Measurement of stresses when the structure performs vibrations according to the eigenmode
Intensity of the static image for the circular polariscope is expressed as:
where $C$ is a product of a constant which depends on the thickness and material of the structure with the difference of principal stresses.
Intensity of the time averaged image for the circular polariscope is expressed as:
where $C$ is a product of a constant which depends on the thickness and material of the structure with the difference of principal stresses in the state of extreme deflections according to the eigenmode, $n$ is a large integer number.
Further the roots of the equation:
are denoted by ${C}_{i}$.
Also the roots of the equation:
are denoted by ${\stackrel{}{C}}_{i}$.
Variations of intensities as functions of $C$ are presented in Fig. 1. Variations of derivatives of intensities with respect to $C$ as functions of $C$ are presented in Fig. 2. Variation of ${\stackrel{}{C}}_{i}{C}_{i}$ as a function of $i$ is presented in Fig. 3. The values of ${C}_{i}$ and ${\stackrel{}{C}}_{i}$ are presented in Table 1.
Fig. 1. $I$ and $\stackrel{}{I}$ as functions of $C$
Fig. 2. $dI/dC$ and $(dI\mathrm{}\u0305)/dC$ as functions of $C$
Fig. 3. ${\stackrel{}{C}}_{i}{C}_{i}$ as a function of $i$
Table 1. Values of ${C}_{i}$ and ${\stackrel{}{C}}_{i}$
$i$

${C}_{i}$

${\stackrel{}{C}}_{i}$

1

0.785398

1.20241

2

2.35619

2.76004

3

3.92699

4.32686

4

5.49779

5.89577

5

7.06858

7.46546

6

8.63938

9.03553

7

10.2102

10.6058

8

11.781

12.1762

9

13.3518

13.7467

10

14.9226

15.3173

11

16.4934

16.8879

12

18.0642

18.4585

13

19.635

20.0292

14

21.2058

21.5999

15

22.7765

23.1706

16

24.3473

24.7413

17

25.9181

26.312

18

27.4889

27.8828

19

29.0597

29.4535

20

30.6305

31.0242

In the previous paper the data which is necessary to interpret experimental results of time averaged photoelasticity were obtained on the basis of analytical investigations based on integrals and using the zeroth order Bessel function of the first kind. The results obtained in this paper correspond with the results obtained analytically in the previous paper and the numerical procedure does not require sophisticated mathematical techniques.
2.2. Measurement of stresses when the structure is slowly loaded from the status of equilibrium by linearly increasing the load till its final value
Intensity of the time averaged image for the circular polariscope is expressed as:
where $C$ is a product of a constant which depends on the thickness and material of the structure with the difference of principal stresses at the final value of the load.
Variations of intensities as functions of $C$ are presented in Fig. 4. Variations of derivatives of intensities with respect to $C$ as functions of $C$ are presented in Fig. 5. Variations of the values of ${C}_{i}$ and ${\stackrel{}{C}}_{i}$ as functions of $i$ are presented in Fig. 6. The values of ${C}_{i}$ and ${\stackrel{}{C}}_{i}$ are presented in Table 2.
Fig. 4. $I$ and $\stackrel{}{I}$ as functions of $C$
Fig. 5. $dI/dC$ and $(dI\mathrm{}\u0305)/dC$ as functions of $C$
Fig. 6. ${C}_{i}$ and ${\stackrel{}{C}}_{i}$ as functions of $i$
Table 2. Values of ${C}_{i}$ and ${\stackrel{}{C}}_{i}$
$i$

${C}_{i}$

${\stackrel{}{C}}_{i}$

1

0.785398

1.5708

2

2.35619

3.14159

3

3.92699

4.71239

4

5.49779

6.28319

5

7.06858

7.85398

6

8.63938

9.42478

7

10.2102

10.9956

8

11.781

12.5664

9

13.3518

14.1372

10

14.9226

15.708

11

16.4934

17.2788

12

18.0642

18.8496

13

19.635

20.4204

14

21.2058

21.9911

15

22.7765

23.5619

16

24.3473

25.1327

17

25.9181

26.7035

18

27.4889

28.2743

19

29.0597

29.8451

20

30.6305

31.4159

Thus the numerical procedure enables to obtain the data required for the interpretation of photoelastic measurements without the need of complicated mathematical techniques, which could be based on the use of the generalized zeroth order Bessel function of the first kind.
From the obtained results a constant shift ${\stackrel{}{C}}_{i}{C}_{i}=$ 0.785398 between the corresponding values of the roots of equations is observed from the data presented in the Table. Of course in order to prove if this is exactly true the strict mathematical investigation based on the generalized zeroth order Bessel function of the first kind would be required.
3. Experimental measurements of stresses in polymeric films
Qualitative investigations of stresses of samples of LDPE films were performed by taking into account the level of stresses in unloaded samples as well as in samples experiencing tensile loading. Samples of LDPE films having various characteristics were analyzed, they had the thickness $\delta $ varying from 8 μm up to 180 μm. In order to obtain photoelastic images representing stress distributions in the investigated polymeric films the experimental setup with „General Purpose Strain Viewer“ shown in Fig. 7 was used. Photoelastic images representing stress distributions were registered by using the digital camera EO1312c. Some of the obtained results are presented in Fig. 8.
From the obtained results of experimental investigations one can see that only when the thicknesses of the film are 150 µm and 180 µm in the unloaded samples of the films there are stresses which occured in the process of production of the films. While in the films of smaller thicknesses there are no observable stresses from the process of production of the films. With the increase of the thickness of the films of LDPE type in the loaded samples higher order photoelastic fringes are observed. They enable to interpret stress distributions in the films.
Fig. 7. View of the experimental setup used for photoelastic stress analysis of LDPE polymeric films: 1 – General Purpose Strain Viewer, 2 – tested material, 3 – USB digital camera EO1312c
Fig. 8. Photoelastic images representing stress distributions of samples of polymeric film of LDPE type of various thicknesses in unloaded and loaded conditions: a), c), e), g), i), k), m) – photoelastic images representing distributions of stresses of samples of unloaded film of LDPE type; b), d), f), h), j), l), n) – photoelastic images representing distributions of stresses of samples of loaded film of LDPE type
a)$\delta =$ 8 µm
b)$\delta =$ 8 µm
c)$\delta =$ 25 µm
d)$\delta =$ 25 µm
e)$\delta =$ 45 µm
f)$\delta =$ 45 µm
g)$\delta =$ 50 µm
h)$\delta =$ 50 µm
i)$\delta =$ 80 µm
j)$\delta =$ 80 µm
k)$\delta =$ 150 µm
l)$\delta =$ 150 µm
m)$\delta =$ 180 µm
n)$\delta =$ 180 µm
4. Conclusions
In the previous paper the data which is necessary to interpret experimental results of time averaged photoelasticity were obtained on the basis of analytical investigations based on integrals and using the zeroth order Bessel function of the first kind. The results obtained in this paper correspond with the results obtained analytically in the previous paper and the numerical procedure does not require sophisticated mathematical techniques.
Numerical procedure of the same type is applied to obtain data which is needed for interpretation of experimental results when the structure is slowly loaded from the status of equilibrium by linearly increasing the load till its final value. Thus the numerical procedure enables to obtain the data required for the interpretation of photoelastic measurements without the need of complicated mathematical techniques, which could be based on the use of the generalized zeroth order Bessel function of the first kind.
From the obtained results a constant shift between the corresponding values of the roots of equations is observed. In order to prove if this is exactly true the strict mathematical investigation based on the generalized zeroth order Bessel function of the first kind would be required.
The obtained results are used in the process of interpretation of stress measurements in photoelastic experiments and a numerical procedure of the proposed type might be applied to other time averaging problems in a similar way.
Experimental measurements of stresses in polymeric films on a specially developed experimental setup have been performed. Qualitative investigations of stresses of samples of LDPE films were performed by taking into account the level of stresses in unloaded samples as well as in samples experiencing tensile loading. Samples of LDPE films having various characteristics were analyzed, they had the thickness varying from 8 μm up to 180 μm.
From the obtained results of experimental investigations one can see that only when the thicknesses of the film are 150 µm and 180 µm in the unloaded samples of the films there are stresses which occured in the process of production of the films. While in the films of smaller thicknesses there are no observable stresses from the process of production of the films. With the increase of the thickness of the films of LDPE type in the loaded samples higher order photoelastic fringes are observed. They enable to interpret stress distributions in the films. This is especially important in the process of operation of the printing device. When the operator of the printing device notices from the photoelastic images that a critical situation is approaching, he is to immediately stop the process of printing and make necessary adjustments.
The obtained results are used in the process of measurements of stresses in the elements of a printing device.
References
 Ragulskis M., Ragulskis L. On interpretation of fringe patterns produced by time average photoelasticity. Experimental Techniques, Vol. 29, Issue 3, 2005, p. 4851. [Search CrossRef]
 Rossini N. S., Dassisti M., et al. Methods of measuring residual stresses in components. Materials & Design, Vol. 35, Issue 3, 2012, p. 572588. [Search CrossRef]
 Parlevliet P., Bersee H. E. N., Beukers A. Residual stresses in thermoplastic composites – a study of the literature – Part II: Experimental techniques. Composites Part A: Applied Science and Manufacturing, Vol. 38, Issue 3, 2007, p. 651665. [Search CrossRef]
 Mittal R. K., Khan A. Effect of various parameters on residual stresses in transparaent polymeric tubes. International Polymer Processing, Vol. 5, Issue 2, 1990, p. 142148. [Search CrossRef]
 Postawa P., Kwiatkowski D. Residual stress distribution in injection molded parts. Journal of Achievements in Materials and Manufacturing Engineering, Vol. 18, Issue 2, 2006, p. 172174. [Search CrossRef]
 Wang T., Young W. B. Study on residual stresses of thinwalled injection molding. European Polymer Journal, Vol. 41, Issue 10, 2005, p. 25112517. [Search CrossRef]
 Karalekas D. E., Agelopoulos A. On the use of stereolithography built photoelastic models for stress analysis investigations. Materials & Design, Vol. 27, Issue 2, 2006, p. 100106. [Search CrossRef]
 Kim S. Y., Kim C. H., et al. Measurement of residual stresses in film insert molded parts with complex geometry. Polymer Testing, Vol. 28, Issue 5, 2009, p. 500507. [Search CrossRef]
 Weng C., Lee W. B., To S. Birefringence techniques for the characterization of residual stresses in injectionmoulded microlens arrays. Polymer Testing, Vol. 28, Issue 7, 2009, p. 709714. [Search CrossRef]
 James M. N., Christoper C. J., Lu Y., Patterson E. A. Fatigue crack growth and crazeinduced crack tip shielding in polycarbonate. Polymer, Vol. 53, Issue 7, 2012, p. 15581570. [Search CrossRef]